synthetic fibres and steel fibres - northumbria research fibres and steel fibres in...citation:...
Post on 05-Apr-2018
Embed Size (px)
Citation: Richardson, Alan and Landless, Sean (2009) Synthetic fibres and steel fibres in concrete with regard to bond strength and toughness. Northumbria Working Paper Series: Interdisciplinary Studies in the Built and Virtual Environment, 2 (2). pp. 128-140. ISSN 1756-2473
Published by: Northumbria University
This version was downloaded from Northumbria Research Link: http://nrl.northumbria.ac.uk/2269/
Northumbria University has developed Northumbria Research Link (NRL) to enable users to access the Universitys research output. Copyright and moral rights for items on NRL are retained by the individual author(s) and/or other copyright owners. Single copies of full items can be reproduced, displayed or performed, and given to third parties in any format or medium for personal research or study, educational, or not-for-profit purposes without prior permission or charge, provided the authors, title and full bibliographic details are given, as well as a hyperlink and/or URL to the original metadata page. The content must not be changed in any way. Full items must not be sold commercially in any format or medium without formal permission of the copyright holder. The full policy is available online: http://nrl.northumbria.ac.uk/policies.html
This document may differ from the final, published version of the research and has been made available online in accordance with publisher policies. To read and/or cite from the published version of the research, please visit the publishers website (a subscription may be required.)
Synthetic fibres and steel fibresin concrete with regard tobond strength and toughness
Alan E Richardson* and Sean Landless*
The ability of fibre reinforced concrete composites to absorb energy has long been
recognised as one of the most important benefits of the incorporation of fibres into plain
concrete (Golpalaratham and Gettu 1995). Steel and synthetic fibres have been used
in concrete floor slabs with success in providing crack control. Slab design using
synthetic fibres relies heavily upon manufacturers design guidance whereas steel fibres
have better developed independent design guides available to assist their correct use
(The Concrete Society 2007a). This paper examines the pull out values of both steel and
Type 2 synthetic fibres embedded in concrete and equates their dosage when used in
beams to provide near equal toughness values, thus providing the designer with a
synthetic/steel fibre ratio by mass of fibre addition for equal performance. According to
Nataraja, et al (2000), the most common method to measure toughness, is to use the
load-deflection curve. One of the most widely used load-deflection tests has been ASTM
1018, which was used herein to evaluate the post crack toughness; by stating
toughness as independent indices and residual strengths based upon the deflection at
the formation of the first crack in the beam in relation to fixed points of further deflections
under load. The ASTM test was chosen as it has been widely used and it is readily
understood by many readers. The research demonstrates that near equal post crack
toughness can be achieved in concrete beams using steel and synthetic fibres, at
Keywords: Steel fibres, synthetic fibres, toughness, beam, load deflection curve.
Built Environment Research Papers December 2009
*School of the Built Environment, Northumbria University, Ellison Building, Newcastle upon Tyne NE1 8ST
This study is a comparative investigation into the bond and toughness effects of Type 2 synthetic fibresand steel fibres using bespoke pull out tests to identify fibre bond strength and then to establish batchingquantities by weight for manufacture of beams for testing to ASTM 1018. The test programme providesan in-depth comparative examination of the effects of these fibres on the concrete beams.
Steel fibres are used in many engineering applications to great effect in controlling cracking of the concreteand enhancing toughness. Steel has a natural affinity with concrete as good bond strength can be developedand the coefficient of expansion for steel and concrete are virtually identical. The steel fibres selected forthis study were 50mm long by 1 mm diameter with a tensile strength of 1100 MPa with offset ends toenhance the pull out strength.
Macro synthetic fibres have been added to concrete since the mid-1980s, (Concrete Society TechnicalReport 65). However, there is still some debate as to the benefits that they can offer the designer and enduser. Manufacturers are making claims for their products that would benefit from independent researchto identify and quantify the properties and performance claimed. This view is supported by TechnicalReport 65 which states, Much development of the use of Type 2 fibres has been by individualmanufacturers, supported by a limited amount of published research. There are an increasing number ofapplications, and some projects have appeared in the trade and technical literature, although very little ofthis is peer reviewed.
Synthetic fibres for use in concrete are classified in BS EN 14889-2. They fall into two categories: Type1 (Monofilament < 0.3 mm diameter); and, Type 2 (Macro Synthetic > 0.3 mm diameter). The fibres asused in this study have the following properties: dimensions of 40 mm x 1.67 mm x 0.095 mm, modulusof elasticity of 9.5GPa, a tensile strength of 620MPa, and they are composed of 90% polypropylene and10% polyethylene.
According to Kiss (2008), it is likely that the market would be more relaxed about expanding its usage [offibres in concrete], if independent guidance were available to cover aspects such as design, constructionand performance in service. This work goes some way in achieving this goal.
According to Bentur and Mindness (2007) No standard tests are available for fibre pull outcharacteristics. However single fibre pullout was adopted in place of multiple fibre pull out, to reducethe variables of fibre orientation and eccentric loading.
The test was to be carried out in two parts, the first being fibre pull out tests to establish the bond strengthof each fibre, the second part was a three point loading test to establish flexural strength and toughnessusing beams of each fibre type.
According to Golpalaratham and Gettu (1995), the flexural test is most popular because it simulates morerealistically the conditions in many practical situations and the research follows this guidance.
Three test cubes, of two fibre types (6 cubes in total) were formed with six fibres embedded to half of theirlength and cured for 28 days prior to pull out testing to establish bond strength (See Figures 1 and 2).Single fibres were loaded until pull out failure occurred and the final pull out force was recorded. Theprocedure was to add weight by 0.1kg for synthetic samples and 1.0 kg for steel samples, at 60 secondintervals, until pull-out failure occurred. Creep was noticed with some of the synthetic fibres and nofurther load was added at this point. Failure occurred usually within two minutes from this point.
Using the pull out data, the steel and synthetic fibre bond strength performance was examined to establishrelative fibre dosage per beam type.
Golpalaratham and Gettu (1995) state, most standards are comparable, as ACI 544 uses a ratio of
Synthetic fibres and steel fibres in concrete with regard to bond strength and toughness
Built Environment Research Papers Vol. 2 No. 2, 2009
Built Environment Research Papers December 2009
Figure 1 G clamp providing a plane clamp for fibre pull out
Figure 2 Steel fibre under pull out load
load/deflection curve so does ASTM 1018, which is essentially the same, however the limiting deflectionanalysis in ASTM 1018 was considered a most useful quality for a paired comparison test.
Six 100 x 100 x 500 mm beams were cast with each fibre type (12 in total) and they were tested to ASTMC1018 to provide flexural strength, first crack load and toughness data, using a three point loadingconfiguration as shown in Figure 3.
Stahli and Mier (2007) comment that the fibres tend to align along the walls of the moulds and it can beshown that these highly reinforced surface layers add significantly to the strength of the beam. This effectof fibre orientation applies equally to both beams, although synthetic fibres will be greatly affected by theconcrete viscosity and aggregate size.
Whole beams were used rather than cut beams because according to Stahli and Mier (2007), no significantdifference was observed in the fracture process between moulded and cut specimens and given fibreswhen cast, tend to align along the walls of the mould, this quality was sought to produce the mostrepresentative test conditions of concrete when cast against formwork.
Formula for flexural strength
R = 3Pa (from ASTM C78)bd2
P= applied load, a= distance between line of fracture and nearest support,
b= average width of beam, d= average depth of beam, L = span length
In accordance with ASTM C 1018, the toughness indices (I) and residual strength values (R) are calculatedas follows:
Determine the first-crack deflection as the deflection corresponding to the length OB in Figure 3.Determine the area under the load-deflection curve up to the first-crack deflection, i.e. the triangulararea OAB.
Determine the area under the load-deflection c